*where G is the shear modulus, the slope of the linear elastic region of the shear*
stress–strain curve. Table 7.1 also gives the shear moduli for a number of the
common metals.

**7.4 A**

**NELASTICITY**

Up to this point, it has been assumed that elastic deformation is time independent, that is, that an applied stress produces an instantaneous elastic strain that remains constant over the period of time the stress is maintained. It has also been assumed that upon release of the load the strain is totally recovered, that is, that the strain immediately returns to zero. In most engineering materials, however, there will also exist a time-dependent elastic strain component. That is, elastic deformation will continue after the stress application, and upon load release some finite time is required for complete recovery. This time-dependent elastic behavior is known as

**anelasticity, and it is due to time-dependent microscopic and atomistic processes**

that are attendant to the deformation. For metals the anelastic component is nor-
mally small and is often neglected. However, for some polymeric materials its
magnitude is significant; in this case it is termed*viscoelastic behavior,*兵which is the
discussion topic of Section 7.15.其

**E**

**XAMPLE**

**P**

**ROBLEM**

**7.1**

A piece of copper originally 305 mm (12 in.) long is pulled in tension with a stress of 276 MPa (40,000 psi). If the deformation is entirely elastic, what will be the resultant elongation?

**S**

**O L U T I O N**

Since the deformation is elastic, strain is dependent on stress according to
Equation 7.5. Furthermore, the elongation⌬*l is related to the original length*
*l0* through Equation 7.2. Combining these two expressions and solving for

⌬*l yields*

⫽ ⑀*E*⫽

### 冉

⌬*l*

*l0*

### 冊

*E*

⌬*l*⫽*l*0
*E*

The values of *and l*0 are given as 276 MPa and 305 mm, respectively, and

*the magnitude of E for copper from Table 7.1 is 110 GPa (16* ⫻ 106 _{psi).}

Elongation is obtained by substitution into the expression above as

⌬*l*⫽(276 MPa)(305 mm)

110⫻103_{MPa} ⫽0.77 mm (0.03 in.)

**7.5 E**

**LASTIC**

**P**

**ROPERTIES OF**

**M**

**ATERIALS**

When a tensile stress is imposed on virtually all materials, an elastic elongation
and accompanying strain⑀*z*result in the direction of the applied stress (arbitrarily

*there will be constrictions in the lateral (x and y) directions perpendicular to the*
applied stress; from these contractions, the compressive strains ⑀*x* and ⑀*y* may be

*determined. If the applied stress is uniaxial (only in the z direction), and the material*
is isotropic, then⑀*x* ⫽ ⑀*y***. A parameter termed Poisson’s ratio** is defined as the

ratio of the lateral and axial strains, or

⫽ ⫺ ⑀*x*

⑀*z*

⫽ ⫺ ⑀*y*

⑀*z*

(7.8)

The negative sign is included in the expression so that will always be positive,
since ⑀*x* and ⑀*z* will always be of opposite sign. Theoretically, Poisson’s ratio for

isotropic materials should be ; furthermore, the maximum value for (or that value for which there is no net volume change) is 0.50. For many metals and other alloys, values of Poisson’s ratio range between 0.25 and 0.35. Table 7.1 shows values for several common materials; a more comprehensive list is given in Table B.3, Appendix B.

For isotropic materials, shear and elastic moduli are related to each other and to Poisson’s ratio according to

*E*⫽*2G(1*⫹) (7.9)

*In most metals G is about 0.4E; thus, if the value of one modulus is known, the*
other may be approximated.

Many materials are elastically anisotropic; that is, the elastic behavior (e.g., the
*magnitude of E) varies with crystallographic direction (see Table 3.7). For these*
materials the elastic properties are completely characterized only by the specification
of several elastic constants, their number depending on characteristics of the crystal
structure. Even for isotropic materials, for complete characterization of the elastic
properties, at least two constants must be given. Since the grain orientation is
random in most polycrystalline materials, these may be considered to be isotropic;

**158** ● **Chapter 7 / Mechanical Properties**

*z*
*y*
*x*
*l*_{0}_{z}*z*
*z*
⌬*lz*
2
⌬*lx*
2
*z*
⑀
2
⌬*lz*/2
*l*_{0}_{z}*=*
⫺⑀*x*
2
⌬*lx*/2
*l*_{0}_{x}*=*
*l*_{0}_{x}

**FIGURE7.9** *Axial (z) elongation*

*(positive strain) and lateral (x and y)*
contractions (negative strains) in
response to an imposed tensile stress.
Solid lines represent dimensions after
stress application; dashed lines, before.

**7.5 Elastic Properties of Materials** ● **159**

inorganic ceramic glasses are also isotropic. The remaining discussion of mechanical behavior assumes isotropy and polycrystallinity (for metals and crystalline ceramics) because such is the character of most engineering materials.

**E**

**XAMPLE**

**P**

**ROBLEM**

**7.2**

A tensile stress is to be applied along the long axis of a cylindrical brass rod
that has a diameter of 10 mm (0.4 in.). Determine the magnitude of the load
required to produce a 2.5 ⫻ 10⫺3 _{mm (10}⫺4 _{in.) change in diameter if the}

deformation is entirely elastic.

**S**

**O L U T I O N**

This deformation situation is represented in the accompanying drawing.

*When the force F is applied, the specimen will elongate in the z direction and*
at the same time experience a reduction in diameter,⌬*d, of 2.5*⫻10⫺3_{mm in}

*the x direction. For the strain in the x direction,*

⑀*x*⫽ ⌬
*d*
*d0* ⫽ ⫺
2.5⫻10⫺3_{mm}
10 mm ⫽ ⫺2.5⫻10
⫺4

which is negative, since the diameter is reduced.

*It next becomes necessary to calculate the strain in the z direction using*
Equation 7.8. The value for Poisson’s ratio for brass is 0.34 (Table 7.1), and thus

⑀*z*⫽ ⫺ ⑀*x*

⫽ ⫺

(⫺2.5⫻10⫺4_{)}

0.34 ⫽7.35⫻10

⫺4

The applied stress may now be computed using Equation 7.5 and the modulus
of elasticity, given in Table 7.1 as 97 GPa (14⫻106_{psi), as}

⫽ ⑀*zE*⫽(7.35⫻10⫺4)(97⫻ 103MPa)⫽71.3 MPa
*z*
*F*
*F*
*x*
*d*_{0}
*d _{i}*

*l*0

*li*⑀

*z*⌬

*0*

_{l}l*li*⫺

*l*0

*l*0 = ⑀

*x*⌬

*0*

_{d}d*di*⫺

*d*0

*d*0 = = =

Finally, from Equation 7.1, the applied force may be determined as
*F*⫽*A0*⫽

### 冉

*d*0 2

### 冊

2 앟 ⫽(71.3⫻106_{N/m}2

_{)}

### 冉

10⫻10⫺ 3_{m}2

### 冊

2 앟⫽5600 N (1293 lbf)### M E C H A N I C A L B E H A V I O R — M E T A L S

For most metallic materials, elastic deformation persists only to strains of about
0.005. As the material is deformed beyond this point, the stress is no longer
proportional to strain (Hooke’s law, Equation 7.5, ceases to be valid), and
* permanent, nonrecoverable, or plastic deformation occurs. Figure 7.10a plots*
schematically the tensile stress–strain behavior into the plastic region for a
typical metal. The transition from elastic to plastic is a gradual one for most
metals; some curvature results at the onset of plastic deformation, which increases
more rapidly with rising stress.

From an atomic perspective, plastic deformation corresponds to the breaking of bonds with original atom neighbors and then reforming bonds with new neighbors as large numbers of atoms or molecules move relative to one another; upon removal of the stress they do not return to their original positions. This permanent deforma- tion for metals is accomplished by means of a process called slip, which involves the motion of dislocations as discussed in Section 8.3.

**7.6 T**

**ENSILE**

**P**

**ROPERTIES**